High strain rate characterization of shock absorbing ... strain rate characterization of shock ......
Embed Size (px)
Transcript of High strain rate characterization of shock absorbing ... strain rate characterization of shock ......
Shock and Vibration 10 (2003) 179186 179IOS Press
High strain rate characterization of shockabsorbing materials for landmine protectionconcepts
Jennifer McArthura, Christopher Salisburya, Duane Cronina, Michael Worswicka and Kevin WilliamsbaUniversity of Waterloo, 200 University Ave W., Waterloo, ON, Canada N2L 3G1Tel.: +1 519 888 4567 x 2346; E-mail: firstname.lastname@example.orgDefence Research Establishment Valcartier, 2459 Pie XI Blvd. Nord, Val B elair, Quebec, Canada G3J 1X5
Received 3 December 2001
Revised 17 October 2002
Abstract. Numerical modelling of footwear to protect against anti-personnel landmines requires dynamic material properties inthe appropriate strain rate regime to accurately simulate material response. Several materials (foamed metals, honeycombs andpolymers) are used in existing protective boots, however published data at high strain rates is limited.Dynamic testing of several materials was performed using Split Hopkinson Pressure Bars (SHPB) of various sizes and materials.The data obtained from these tests has been incorporated into material models to predict the initial stress wave propagationthrough the materials. Recommendations for the numerical modeling of these materials have also been included.
An estimated 110 million landmines are hiddenaround the world , interfering with agriculture aswell as industrial development. In 1997, the Ottawatreaty  was signed to ban landmines around theworld and many nations have responded to this prob-lem with extensive de-mining efforts to decontaminatemine-affected areas.
The design of footwear to protect against landminesis extremely complex and must take into account boththe shock waves from the blast and the rapid expansionof the explosive gases immediately below the foot. Ex-perimental testing is limited since it is extremely expen-sive and requires significant expertise. A method thatallows many concepts to be inexpensively comparedand ranked prior to the experimental trials is thus de-sirable. With such a method, many potential conceptsmay be evaluated and only those that show the mostpromise would then be tested experimentally. Numer-ical modelling allows for the evaluation of many con-cepts at a lower cost. To ensure that numerical mod-
els will be realistic, several simpler models have beenanalysed and validated with experimental results . These models found that the explosive gases ex-pand at speeds as high as 1800 m/s. Since the footwearmust be thin enough for normal motion, the peak strainrates in the material will be very high and thus materialproperties obtained at these strain rates are desired.
This paper discusses the testing and modeling of var-ious materials that are used in existing protective bootsusing the Split Hopkinson Bar method. These mate-rials include closed-cell polyethylene foams, open-cellaluminum foams and honeycombs and polyurethanerubber.
2. Literature review
2.1. Material models shock behaviour
The LS-DYNA hydrocode contains many materialmodels representing a variety of materials . Ide-ally, both shock and deviatoric behaviour should be in-
ISSN 1070-9622/03/$8.00 2003 IOS Press. All rights reserved
180 J. McArthur et al. / High strain rate characterization of shock absorbing materials for landmine protection concepts
Striker Incident Bar Transmitter Bar
Fig. 1. Set-up of compressive split Hopkinson bar (not to scale).
corporated into the material models. Shock may beaccounted for by the use of an equation of state andthere are few models that allow this equation of stateto be added. The simplest of these models include thenull material model which assumes that the material isa viscous fluid and neglects deviatoric properties, theelastic-plastic-hydrodynamic model that assumes thematerial follows a straight elastic curve to yielding andthen may have some strain hardening or softening in theplastic region. Neither accounts for extensive deforma-tion, however and a deviatoric model should be used todetermine the long-term deformation of any material.
The linear polynomial equation of state  may beused with the data tabulated in LASL shock hand-book  to describe the shock behaviour.
2.2. Material models deviatoric behaviour
This paper contains stress-strain curves that may beincorporated into deviatoric material models. The fol-lowing models are recommended for the materials dis-cussed in this report.
Honeycombs and brittle foamsThe honeycomb model  uses the solid material
properties, densification strain and orthotropic loadcurves in compression to determine deviatoric be-haviour of the material. Isotropic materials such asbrittle foams may also use this material model and onlytwo load curves (uniaxial compression and shear) needto be defined in this case.
Nearly incompressible rubber materials (polyurethane)
The Mooney-Rivlin rubber model is a two-parametermodel for nearly incompressible rubber materials .The input data includes density, Poissons ratio and aload curve (either force-displacement or stress-strain)which it uses to calculate the two parameters A andB. This model, with an appropriate strain-rate curveat the expected strain rates, has been used for model-ing polyurethane rubber response to blast loading withsome success .
Polymer foamsThe simplest foam-specific model is the crushable
foam material model . The inputs for this model arethe initial density of the foam and a stress-strain curveat a given strain rate.
2.3. Split hopkinson bars for testing low-impedancematerials
The Hopkinson Bar is the most commonly usedmethod for testing materials in the strain rate regime of102104 s1. Only compressive split Hopkinson Bar(CSHB) tests were used.
The CSHB consists of a striker bar, an incident barand a transmitter bar, shown in Fig. 1. The striker baris propelled from a gas gun at a desired velocity andimpacts the incident bar. A compressive stress waveis imparted into the incident bar and propagates un-interrupted until it reaches the sample. The wave ispartially transmitted through the sample into the trans-mitter bar and the rest is reflected into the incident bar.Strain gauges record the strain-time history of both theincident, reflected and transmitted waves.
Classical analysis of a split Hopkinson Bar requiresthe following assumptions : (i) the bars must remainelastic throughout the test; (ii) no attenuation or disper-sion of the stress waves occur; (iii) the pulse is uniformover the cross-section of the bar and, (iv) the specimenremains in equilibrium throughout the test. These as-sumptions must be valid in order to apply the classicalHopkinson bar equations (Eqs (1)(4)) to determine thetime histories of stress, strain and strain rate within thespecimen.
(t) :=2 CbLs
(t) :=2 CbLs
(t) :=2 CbLs
3. Experimental methods
Where Cb is the speed of sound inside the bars, Ebis the modulus of elasticity of the bars, b is the densityof the bars, Ab and As are the cross-sectional areas of
J. McArthur et al. / High strain rate characterization of shock absorbing materials for landmine protection concepts 181
Table 1Sample sizes and maximum loading for low-rate material tests
Material Sample size (w x d x l) Aspect ratio (w:l) Strain rate
34 kg/m3 polyethylene foam (HL34) 10 cm 10 cm 10 cm 1:1 0.03/s34 kg/m3 polyethylene foam (LD24) 10 cm 10 cm 3.2 cm 1:3 0.03/sPolyurethane rubber 5 cm 5 cm 1 cm 1:5 0.01/sOpen-cell Al Foam (7% density, 10PPI) 3.8 cm 3.6 m 1.2 cm 1: 3.170.01/sOpen-cell Al Foam (7% density, 20PPI) 3.9 m 3.9 m 1.3 cm 1:3 0.01/sOpen-cell Al Foam (7% density, 40PPI) 3.9 cm 3.75 cm 1.3 cm 1:2.95 0.01/sOpen-cell Al Foam (11% density, 10PPI) 2.5 cm 2.2 cm 1.8 cm 1:1.3 0.01/sAluminum Honeycomb (ACG) 10 cm 10 cm 1.6 mm 1:6.25 0.03/sAluminum Honeycomb (CR-III) 5 cm 5 cm 1.6 mm 1:3.125 0.03/s
0 0.2 0.4 0.6 0.8 1
Fig. 2. Stress-strain behaviour of HL34 foam.
the bars and specimen, Ls is the length of the specimenand r and t are reflected and transmitted strains.
It should be noted that the real behaviour of the barsis more complex than assumed. Friction must be over-come before a specimen can expand or contract radi-ally. Davies  suggests certain criteria for specimendimensions to minimize this effect. Aspect ratios arevery important for ensuring that the friction effects atthe ends is minimal , and were kept at L/D = 1for the majority of the materials tested. In order tomeasure higher strain rates, the aspect ratio of the alu-minum foam and honeycomb specimens were as lowas L/D = 0.25. This was acceptable because these ma-terials exhibit very low Poissons ratios (approximately0.05 ) and thus do not deform significantly in theradial direction, so the frictional effects were much lesssignificant than for the other materials.
Polymeric bars require a different approach. Ba-con  developed an experimental method to correctfor the attenuation and dispersion of the wave as it prop-agates along the length of the bar. The method is basedon performing a free end test (where the end of thebar is not restricted) while measuring the incident andreflected wave. Since the bar is allowed to move freely
0 0.2 0.4 0.6 0.8 1
Fig. 3. Stress-strain behaviour of LD24 foam.
at the interface end the entire wa